- About this Journal
- Abstracting and Indexing
- Aims and Scope
- Article Processing Charges
- Articles in Press
- Author Guidelines
- Bibliographic Information
- Citations to this Journal
- Contact Information
- Editorial Board
- Editorial Workflow
- Free eTOC Alerts
- Publication Ethics
- Submit a Manuscript
- Table of Contents
Volume 2012 (2012), Article ID 871208, 4 pages
Synthesis of Cobalt-Encapsulated Carbon Nanocapsules Using Cobalt-Doped Fullerene Nanowhiskers
1Institute of Materials Science, Graduate School of Pure and Applied Sciences, University of Tsukuba, Ibaraki Tsukuba, 305-8753, Japan
2Fullerene Engineering Group, Advanced Materials Processing Unit, National Institute for Materials Science, Namiki, Ibaraki Tsukuba, 305-0044, Japan
Received 24 December 2011; Accepted 11 January 2012
Academic Editors: C. S. Casari and Y. Song
Copyright © 2012 Daisuke Matsuura et al. This is an open access article distributed under the Creative Commons Attribution License, which permits unrestricted use, distribution, and reproduction in any medium, provided the original work is properly cited.
We synthesized cobalt- (Co-) doped C60 nanowhiskers (NWs) by applying a liquid-liquid interfacial precipitation method using a C60-saturated toluene solution and 2-propanol with Co nitrate hexahydrate (Co(NO3)3·6H2O). Heating the NWs at 873–1173 K produced carbon nanocapsules (CNCs) that encapsulated Co clusters with a hexagonal-closed-packed structure. After heating at 1273 K, the encapsulated Co clusters in CNCs were transformed into orthorhombic Co2C clusters. It was found that Co- and Co2C-encapsulated CNCs can be produced by varying heating temperature.
Carbon nanocapsules (CNCs), which are hollow multiwalled graphitic nanoparticles, exhibit high chemical and thermal stabilities [1–8]. The encapsulation of metallic and carbide clusters in CNCs leads to the formation of catalysts and drug delivery components [4, 9–17]. Such pristine and encapsulated CNCs have been synthesized by arc discharge, chemical vapor deposition, electron irradiation, and thermal decomposition [1, 3–5, 9, 11, 13–15]. Recently, a new synthesis method for CNCs using single-crystal fullerene nanowhiskers (NWs) has been developed by Asaka et al. and Kizuka et al. [18–22]. Fullerene NWs have been synthesized by liquid-liquid interfacial precipitation (LLIP) methods. Metal elements can be doped in fullerene NWs using C60 derivatives and additives in solutions [23–31]. It is expected that the alloying of CNCs and metals can be performed using such metal-doped fullerene NWs. Some of magnetic materials, for example, cobalt (Co) and iron, form solid solutions with carbon. It is expected that various systems with crystal structures, solid solutions, and intermetallics are combined with CNCs. In this study, we demonstrate the synthesis of Co-doped C60 NWs and CNCs encapsulating Co-based clusters.
We synthesized Co-doped C60 NWs using the LLIP method [25–27]. C60 powders were dissolved in toluene to prepare a C60-saturated solution with a solubility of 2.8 g/L. Co nitrate hexahydrate (Co(NO3)3·6H2O) was dissolved in 2-propanol. The C60 toluene solution was poured into a glass vial, and the 2-propanol dissolving Co(NO3)3·6H2O was then added to form a liquid-liquid interface. After the vial was maintained at 278 K for one week, the solution was filtered to extract precipitates. The precipitates were dried and heated in high vacuum at 773–1273 K for 1 h. The rate of temperature increase was 10 K/min. The cooling of the specimens was performed by furnace cool. After cooling, the specimens were dispersed on microgrids and observed by transmission electron microscopy.
3. Results and Discussion
Figure 1 shows a bright field image of an as-precipitated C60 NW. The diameter of as-precipitated C60 NWs ranged from 190 to 940 nm with an average of 440 nm. Electron diffraction showed that the NWs had a tetragonal lattice. The surfaces of the Co-doped NWs are porous, as shown in Figure 1. This feature is similar to Ni-doped NWs , whereas pure C60 NWs are surrounded by plane surfaces [25–27]. Miyazawa and Suga used C60 derivatives in LLIP methods and showed that the crystal growth of C60-derivative NWs is inhibited . Therefore, the porous surfaces of the as-precipitated NWs in this study are attributed to the addition of Co(NO3)36H2O. No Co clusters were observed in the as-precipitated NWs, indicating that the doped Co component is mixed with atomic states in the NWs.
After heating the as-precipitated specimens at 773 K, the shape of the NWs was similar to that of the as-precipitated specimen. After heating at 873 K, the structure of a portion of the NWs was transformed from a tetragonal to an amorphous form. After heating at temperatures higher than 973 K, all NWs were transformed into amorphous forms, and CNCs were observed in the amorphous regions.
Figure 2(a) shows a high-resolution image of a CNC in the specimen heated at 1073 K. The outer graphitic layers of the CNC were three-dimensionally closed, and a cluster was encapsulated. As shown in Figure 2(b), selected-area electron diffraction showed that the encapsulated clusters were Co crystals with a hexagonal-closed-packed (hcp) structure having lattice constants of nm and nm. The diameter of the CNCs ranged from 14 to 76 nm with an average of 35 nm. The diameter of the encapsulated Co clusters ranged from 10 to 44 nm with an average of 20 nm. Figure 2(c) shows the enlarged interface between the encapsulated Co cluster and the graphitic layers in the Co-encapsulated CNC depicted in Figure 2(a). The Co cluster directly bonded with the graphitic layers. The lattice spacing of the Co cluster and the graphitc layers depicted in Figure 2(b) were 0.20 nm and 0.34 nm, respectively, corresponding to () of hcp-Co and (002) of graphitic layers, respectively. In the specimens heated at 873–1173 K, Co-encapsulated CNCs were observed. Figure 3 shows the thickness of the graphitic layers in Co-encapsulated CNCs produced by heating at 1073 K against the diameter of the Co clusters. The diameter of the Co clusters ranges from 10 nm to 45 nm. The maximum thickness of the graphitic layers is 20 nm. In Figure 3, although no clear relationship is observed, the graphitic layers seem to increase with the diameter of the Co clusters. If the graphitic layers were formed by deposition of decomposed carbon atoms on the surfaces of the Co clusters, the thickness of the graphitic layers becomes constant with the diameter of the Co clusters at a certain temperature. On the other hand, if the graphitic layers were formed by simple precipitation from the Co clusters, the thickness of the graphitic layers is proportional to the volume of the Co clusters, that is, the cube of the diameter. Thus, the distribution in Figure 3 suggests that the precipitation of carbon atoms from the Co clusters contributes to the formation of the graphitic layers.
Figure 4(a) shows a high-resolution image of CNCs in the specimen heated at 1273 K. As was the case with the specimens heated at 1073 K, the graphitic layers of the CNCs were closed. Selected-area electron diffraction revealed that the encapsulated clusters were Co2C crystals with an orthorhombic lattice with lattice constants of nm, nm, and nm, as shown in Figure 4(b). The lattice spacing of the Co2C cluster and graphitic layers observed in Figure 4(c) were 0.17 nm and 0.34 nm, respectively, corresponding to () of Co2C and (002) of graphitic layers, respectively. In the specimens heated at 1273 K, the diameter of the CNCs ranged from 44 to 66 nm with an average of 54 nm. In addition, the diameter of the Co2C clusters ranged from 29 to 34 nm with an average of 32 nm. These diameters are larger than those of the specimens heated at 1073 K.
Figure 5 shows the changes in the diameters of both CNCs and encapsulated clusters and in the thickness of the graphitic layers in encapsulated CNCs against the heating temperature. Both the diameters and thickness increase with heating temperature.
The synthesis process for encapsulated CNCs is explained as follows. First, Co atoms that were doped by the addition of Co(NO3)3·6H2O in the NWs aggregated to form Co clusters by heating around 873 K. Subsequently, C60 molecules in the NWs decomposed at temperatures higher than 873 K. This temperature is lower than that at which pure C60 molecules decompose (1073–1173 K) . Hence, in the present NWs, it is inferred that the Co clusters acted as catalysts that decrease the decomposition temperature of C60 molecules. Such decomposed carbon atoms dissolved in the Co clusters during heating. Then, during cooling, carbon atoms precipitated on the surfaces of the Co clusters, followed by the formation of graphitic layers, that is, Co-encapsulated CNCs. At higher heating temperatures (1273 K), more C atoms dissolved in the clusters because of increase in the solubility limit. As a result, the Co2C clusters were formed after cooling from 1273 K.
We successfully synthesized Co-doped C60 NWs using the liquid-liquid interfacial precipitation method with the additive Co(NO3)3·6H2O in 2-propanol. Electron microscopy directly showed that Co- and Co2C-encapsulated CNCs were produced by heating the NWs. It was found that the formation of Co- and Co2C-encapsulated CNCs can be controlled by varying the heating temperature.
This study was partly supported by Grants-in-Aid from the Ministry of Education, Culture, Sport, Science, and Technology, Japan (nos. 22310065 and 23651127).
- R. D. Heidenreich, W. M. Hess, and L. L. Ban, “A test object and criteria for high resolution electron microscopy,” Journal of Applied Crystallography, vol. 1, no. 1, pp. 1–19, 1968.
- D. Ugarte, “Curling and closure of graphitic networks under electron-beam irradiation,” Nature, vol. 359, no. 6397, pp. 707–709, 1992.
- Y. Saito, T. Yoshikawa, M. Inagaki, M. Tomita, and T. Hayashi, “Growth and structure of graphitic tubules and polyhedral particles in arc-discharge,” Chemical Physics Letters, vol. 204, no. 3-4, pp. 277–282, 1993.
- Y. Saito, “Nanoparticles and filled nanocapsules,” Carbon, vol. 33, no. 7, pp. 979–988, 1995.
- V. Z. Mordkovich, A. G. Umnov, T. Inoshita, and M. Endo, “The observation of multiwall fullerenes in thermally treated laser pyrolysis carbon blacks,” Carbon, vol. 37, no. 11, pp. 1855–1858, 1999.
- J. S. Yu, S. B. Yoon, Y. J. Lee, and K. B. Yoon, “Fabrication of bimodal porous silicate with silicalite-1 core/mesoporous shell structures and synthesis of nonspherical carbon and silica nanocases with hollow core/mesoporous shell structures,” The Journal of Physical Chemistry B, vol. 109, no. 15, pp. 7040–7045, 2005.
- Z. Li, M. Jaroniec, P. Papakonstantinou et al., “Supercritical fluid growth of porous carbon nanocages,” Chemistry of Materials, vol. 19, no. 13, pp. 3349–3354, 2007.
- J. N. Wang, L. Zhang, J. J. Niu et al., “Synthesis of high surface area, water-dispersible graphitic carbon nanocages by an in situ template approach,” Chemistry of Materials, vol. 19, no. 3, pp. 453–459, 2007.
- R. S. Ruoff, D. C. Lorents, B. Chan, R. Malhotra, and S. Subramoney, “Single crystal metals encapsulated in carbon nanoparticles,” Science, vol. 259, no. 5093, pp. 346–348, 1993.
- Y. Saito, T. Yoshikawa, M. Okuda et al., “Carbon nanocapsules encaging metals and carbides,” Journal of Physics and Chemistry of Solids, vol. 54, no. 12, pp. 1849–1860, 1993.
- M. Tomita, Y. Saito, and T. Hayashi, “LaC2 encapsulated in graphite nano-particle,” Japanese Journal of Applied Physics, vol. 32, no. 2B, pp. L280–L282, 1993.
- T. Hihara, H. Onodera, K. Sumiyama et al., “Magnetic properties of iron in nanocapsules,” Japanese Journal of Applied Physics, vol. 33, no. 1A, pp. L24–L25, 1994.
- Y. Saito, K. Nishikubo, K. Kawabata, and T. Matsumoto, “Carbon nanocapsules and single-layered nanotubes produced with platinum-group metals (Ru, Rh, Pd, Os, Ir, Pt) by arc discharge,” Journal of Applied Physics, vol. 80, no. 5, pp. 3062–3067, 1996.
- F. Banhart, P. Redlich, and P. M. Ajayan, “Irradiation effects in carbon nanostructures,” Chemical Physics Letters, vol. 292, no. 4–6, pp. 554–560, 1998.
- F. Banhart, “Irradiation effects in carbon nanostructures,” Reports on Progress in Physics, vol. 62, no. 8, pp. 1181–1221, 1999.
- A. Vinu, M. Miyahara, V. Sivamurugan, T. Mori, and K. Ariga, “Large pore cage type mesoporous carbon, carbon nanocage: a superior adsorbent for biomaterials,” Journal of Materials Chemistry, vol. 15, no. 48, pp. 5122–5127, 2005.
- K. Ariga, A. Vinu, M. Miyahara, J. P. Hill, and T. Mori, “One-pot separation of tea components through selective adsorption on pore-engineered nanocarbon, carbon nanocage,” Journal of the American Chemical Society, vol. 129, no. 36, pp. 11022–11023, 2007.
- K. Asaka, R. Kato, Y. Maezono, R. Yoshizaki, K. Miyazawa, and T. Kizuka, “Light-emitting filaments composed of nanometer-sized carbon hollow capsules,” Applied Physics Letters, vol. 88, no. 5, Article ID 051914, 3 pages, 2006.
- K. Asaka, R. Kato, K. Miyazawa, and T. Kizuka, “Deformation of multiwalled nanometer-sized carbon capsules,” Applied Physics Letters, vol. 89, no. 19, Article ID 191914, 3 pages, 2006.
- K. Asaka, R. Kato, R. Yoshizaki, K. Miyazawa, and T. Kizuka, “Conductance of carbon nanocapsule junctions,” Physical Review B, vol. 76, no. 11, Article ID 113404, 2007.
- T. Kizuka, R. Kato, and K. Miyazawa, “Structure of hollow carbon nanocapsules synthesized by resistive heating,” Carbon, vol. 47, no. 1, pp. 138–144, 2009.
- T. Kizuka, R. Kato, and K. Miyazawa, “Surface breakdown dynamics of carbon nanocapsules,” Nanotechnology, vol. 20, no. 10, Article ID 105205, 2009.
- K. Miyazawa, A. Obayashi, and M. Kuwabara, “C60nanowhiskers in a mixture of lead zirconate titanate sol-C60 toluene solution,” Journal of the American Ceramic Society, vol. 84, no. 3–12, pp. 3037–3039, 2001.
- K. Miyazawa, “C70 nanowhiskers fabricated by forming liquid/liquid interfaces in the systems of toluene solution of C70 and isopropy/alcohol,” Journal of the American Ceramic Society, vol. 85, no. 5, pp. 1297–1299, 2002.
- K. Miyazawa, Y. Kuwasaki, A. Obayashi, and M. Kuwabara, “C60 nanowhiskers formed by the liquid-liquid interfacial precipitation method,” Journal of Materials Research, vol. 17, no. 1, pp. 83–88, 2002.
- K. Miyazawa, K. Hamamoto, S. Nagata, and T. Suga, “Structural investigation of the C60/C70 whiskers fabricated by forming liquid-liquid interfaces of toluene with dissolved C60/C70 and isopropyl alcohol,” Journal of Materials Research, vol. 18, no. 5, pp. 1096–1103, 2003.
- K. Miyazawa, Y. Kuwasaki, K. Hamamoto, S. Nagata, A. Obayashi, and M. Kuwabara, “Structural characterization of C60 nanowhiskers formed by the liquid/liquid interfacial precipitation method,” Surface and Interface Analysis, vol. 35, no. 1, pp. 117–120, 2003.
- K. Miyazawa, T. Mashino, and T. Suga, “Structural characterization of the C60[C(COOC2H5)2] whiskers prepared by the liquid-liquid interfacial precipitation method,” Journal of Materials Research, vol. 18, no. 11, pp. 2730–2735, 2003.
- K. Miyazawa and T. Suga, “Transmission electron microscopy investigation of fullerene nanowhiskers and needle-like precipitates formed by using C60 and (-C60)Pt(PPh3)2,” Journal of Materials Research, vol. 19, no. 8, pp. 2410–2414, 2004.
- K. Miyazawa and T. Suga, “Transmission electron microscopy investigation of tubular and capsular needlelike crystals of C60 produced by the liquid-liquid interfacial precipitation method,” Journal of Materials Research, vol. 19, no. 11, pp. 3145–3148, 2004.
- M. Sathish, K. Miyazawa, and T. Sasaki, “Preparation and characterization of Ni incorporated fullerene nanowhiskers,” Diamond and Related Materials, vol. 17, no. 4-5, pp. 571–575, 2008.
- S. D. Leifer, D. G. Goodwin, M. S. Anderson, and J. R. Anderson, “Thermal decomposition of a fullerene mix,” Physical Review B, vol. 51, no. 15, pp. 9973–9978, 1995.